Significance and Use
The thermal expansion under load and the 20 to 50 h creep properties of a refractory are useful in characterizing the load bearing capacity of a refractory that is uniformly heated. Directly applicable examples are blast furnace stoves and glass furnace checkers.
1.1 This test method covers the procedure for measuring the linear change of refractory specimens that are subjected to compressive stress while being heated and while being held at elevated temperatures.
1.2 This test method does not apply to materials whose strength depends on pitch or carbonaceous bonds unless appropriate atmospheric control is used (see 7.3).
1.3 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
compressive stress; creep; elevated temperatures; linear change; refractories; thermal dilation; thermal expansion; Creep; Linear thermal expansion; Loading tests--refractories; Refractories (general);
ICS Number Code 81.080 (Refractories)
ASTM International is a member of CrossRef.
Citing ASTM Standards
[Back to Top]